Research Article Microstructure and Mechanical Properties ... Research Article Microstructure and...
Embed Size (px)
Transcript of Research Article Microstructure and Mechanical Properties ... Research Article Microstructure and...
Research Article Microstructure and Mechanical Properties of Mg/2 wt.%SiCp Nanocomposite Fabricated by ARB Process
Zheng Lv, Xueping Ren, Wenjing Wang, Xiaodan Gao, and Wenjie Li
School of Materials Science and Engineering, University of Science and Technology Beijing, Beijing 100083, China
Correspondence should be addressed to Zheng Lv; email@example.com
Received 5 May 2016; Revised 31 August 2016; Accepted 8 September 2016
Academic Editor: Domenico Acierno
Copyright © 2016 Zheng Lv et al.This is an open access article distributed under the Creative CommonsAttribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Magnesium matrix nanocomposites (MMNC, the same below) containing 2wt.% nanosized SiCp were fabricated through accumulative roll bonding (ARB). The microstructure and mechanical properties of Mg/2wt.%SiCp nanocomposites are reported for various ARB cycles. To evaluate microstructure of the nanocomposites, the field emission scanning electron microscope (FE- SEM), X-ray diffractometer (XRD), and transmission electron microscope (TEM) were applied. After fourteen ARB cycles, the nanocomposite showed a homogeneous distribution of reinforcements and a significant reduction in average matrix grain size. Meanwhile, the nanocomposite revealed a higher percentage of recrystallization and lower intensity of basal texture as compared to monolithicMg.Mechanical properties were investigated through tensile andmicrohardness tests.The strength and elastic modulus and microhardness of Mg/2wt.%SiCp were found to be improved significantly from eight ARB cycles and reach maximum values at fourteen ARB cycles. The ultimate tensile strength, yield strength, microhardness, and elastic modulus of Mg/2wt.%SiCp are considerably increased by 17.6%, 61.0%, 72.7%, and 80.8% as compared to raw Mg, respectively.
Magnesiummatrix composites have been extensively applied in many fields, such as aerospace and light metal automotive applications, due to their low density and superior specific properties including strength, stiffness, and creep resistance [1–10]. The necessity of reducing environmental pollution and protecting natural resources also gives rise to the development of magnesium-based composites with superior mechanical properties . It is widely recognized that judi- cious selection of type, size, and fraction of reinforcements assists in realizing enhanced dimensional stability, damping capacity, and elevated temperature properties . An observ- able improvement in both mechanical and other desirable properties can be attributed to the conjoint and interactive influence of the properties of the matrix and reinforcement phase, coupled with the size, shape, orientation, volume frac- tion, and distribution of reinforcement phase in magnesium matrix .
In the past, various types of reinforcements have been used in magnesiummatrix to synthesize composites possess- ing higher strength, while the silicon carbide (SiC) remains
the most commonly selected reinforcement phase. It has been reported that the presence of micron-sized SiCp led to an increase in hardness and modulus of Mg matrix while reducing the ultimate tensile strength [3, 4]. In recent years, lots of literature proved that the use of nanosized rein- forcements promises to affect both ultimate tensile strength and yield strength of Mg matrix favorably [1, 2, 5–10]. Ferkel andMordike manufactured theMMNC containing 3 vol.%SiCp (30 nm) by powder metallurgy. Cao et al. [1, 6] reported that the nano-SiCp reinforced MMNC fabricated by ultrasonic cavitation both enhanced the UTS and YS of the matrix. Nie et al.  synthesized the MMNC containing 1.0 vol.%SiCp (60 nm) via ultrasonic vibration and obtained a significant improvement in UTS and YS. Thakur  fabri- cated the 1% SiCp (50 nm) reinforced MMNC by microwave assisted powdermetallurgy, with the increase inUTSby 7.78% and YS by 9.84%, respectively.
To produce magnesium matrix composites, a number of conventional processes have been introduced that can broadly be categorized in two processes, namely, powder metallurgy (PM, such as microwave assisted PM route [2, 5]) and ingotmetallurgy techniques (IM, such as stirring casting,
Hindawi Publishing Corporation Journal of Nanomaterials Volume 2016, Article ID 6034790, 12 pages http://dx.doi.org/10.1155/2016/6034790
2 Journal of Nanomaterials
squeeze casting, ultrasonic vibration or cavitation [1, 6, 7], and disintegratedmelt deposition [3, 8, 9]). As themost estab- lished severe plastic deformation for the production of sheet metals, accumulative roll bonding (ARB) processes have been utilized for the synthesis ofmetal matrix composites in recent years [11–19]. The repeated stacking and rolling process offer the possibility of producingmaterials with tailored properties by producing sandwich-like laminates or introducing phases like particles or films . In nanocomposites produced by ARB, well dispersion of nanoparticles could, in theory, be always achieved in the case of sufficient ARB cycles. Fur- thermore, conventional synthesis process and hot working process of MMNC could be integrated through ARB process. ARB processes have been successfully utilized to produce aluminummatrix composites [12–16] or nanocomposites [11, 17, 18]. Yoo et al.  have published the report on AZ31- 0.06 vol.% CNT nanocomposites fabricated by 4-cycle ARB process. But, till date, no report is available on the Mg-SiCp nanocomposites produced by ARB process.
The present work focuses on the Mg/SiCp nanocompos- ites produced by ARB process.The objective of the study is to manufacture finely dispersed Mg/2wt.%SiCp nanocompos- ites with superior mechanical properties by ARB process. A novel method for incorporation of nanosized reinforcements was adopted by ultrasonic-assisted liquid phase deposition, and hot pack rolling was applied in each ARB cycle. The microstructure evolution and mechanical properties of the produced nanocomposites are investigated.
2. Experimental Procedure
2.1. Materials. The annealed sheets of industrial pure mag- nesium (>99.5%) with a dimension of 125 × 55 × 1mm were used as rolled samples. Analytical grade of SiC powder with an average size of 50 nmwas used as reinforcement (Figure 1). The raw Mg sheets had an average grain size of 14.7 𝜇m, as shown in Figure 2. The ultimate tensile strength (UTS), yield strength (YS), elastic modulus (𝐸), andmicrohardness of raw Mg sheet are 247.4MPa, 155.9MPa, 35.9GPa, and 46.6HV, respectively.
2.2. Preparation. Before ARB, the surfaces of Mg sheets were cleaned and degreased. These sheets were scratch brushed with the stainless steel brush and then degreased in acetone. For first ARB cycle, six layers of raw Mg sheets were stacked, and SiC nanoparticles were dispersed on one side of each of the inner four sheets. In present work, the incorporation of SiC nanoparticles was achieved by employing stabilized particle suspended liquids and applying these from the liquid phase to the metal surface through ultrasonic-assisted liquid phase deposition. Each deposition process was the same and was restricted to one sheet. The block copolymer Disperbyk- 2150 (BYK Chemie GmbH) was first dissolved in ethanol, and then the weighed SiC nanoparticles were added to the as-prepared solution. The block copolymer Disperbyk- 2150 is a good dispersing agent to improve the dispersion of nanoparticles in ethanol and stabilize the suspension of the nanoparticles. This mixture was put into an ultrasonic bath and ultrasonicated for 30min at least. After adding Mg
Figure 1: TEMmicrograpy of SiC nanoparticles used in this work.
Figure 2: EBSD grain boundary map of the raw magnesium sheet. RD-ND section with RD parallel to scale bar.
sheet, the suspended liquid was further ultrasonicated until the ethanol was evaporated. Six layers of Mg sheets were stacked together and then were assembled with the self- designed rolling pack. In order to prevent the reaction or bonding between Mg sheets and pack, the outside of each of the outer two Mg sheets was applied to antisolder flux. The schematic diagram of a self-designed rolling pack is presented in Figure 3. The rolling pack is comprised of four 6061 aluminum alloy plates with dimensions of 160 × 96 × 1mm and 160 × 20 × 6mm. The pack is rigidly fixed with blind rivets at the front end and fastened with steel wire at the tail end. There are six holes for riveting at front end and two holes for fastening at tail end.
2.3. ARB Process. The roll bonding process was carried out with no lubrication, using a two-high experimental rolling mill provided by the Engineering Research Institute of USTB (University of Science and Technology Beijing). The rolls were designed with 350mm diameter and 550mm barrel length. The as-prepared material was heated to 673K for
Journal of Nanomaterials 3
Figure 3: The schematic diagram of self-designed rolling pack for ARB process.
30min and then subjected to a series of rolling with 50% reduction and the speed of 1m/min. After rolling, the pack was manually disassembled. This cycle was named one ARB cycle. Subsequently, the nanocomposite sheet was cut into two halves, scratch brushed, degreased in acetone, and stacked over each other, without incorporation of nanoparti- cles between them. The rolling pack and antisolder flux were employed in each ARB cycle.The cyclic ARB process was car- ried out for up to 14 cycles. To compare the microstructural evolution andmechanical properties,monolithicMgwas also prepared with the same process.
2.4. Characterization. The RD-ND planes